#------------------------------------------------------------------------------
#$Date: 2019-11-08 01:32:27 +0200 (Fri, 08 Nov 2019) $
#$Revision: 224511 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/70/06/7700698.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7700698
loop_
_publ_author_name
'Chai, Dongfeng'
'Xin, Jianjiao'
'Li, Bonan'
'Pang, Haijun'
'Ma, Huiyuan'
'Li, Kunqi'
'Xiao, Boxin'
'Wang, Xinming'
'Tan, Lichao'
_publ_section_title
;
 Mo-Based crystal POMOFs with a high electrochemical capacitor
 performance.
;
_journal_issue                   34
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              13026
_journal_page_last               13033
_journal_paper_doi               10.1039/c9dt02420d
_journal_volume                  48
_journal_year                    2019
_chemical_formula_moiety         '0.5(C96 H96 Cu4 Mo24 N48 O78 P2)'
_chemical_formula_sum            'C48 H48 Cu2 Mo12 N24 O39 P'
_chemical_formula_weight         2894.38
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_audit_block_doi                 10.5517/ccdc.csd.cc21tn9v
_audit_creation_date             2019-06-03
_audit_creation_method
;
Olex2 1.2
(compiled 2014.07.22 svn.r2960 for OlexSys, GUI svn.r4862)
;
_audit_update_record
;
2019-06-03 deposited with the CCDC.    2019-07-29 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 107.46(2)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.953(6)
_cell_length_b                   15.982(8)
_cell_length_c                   24.080(10)
_cell_measurement_reflns_used    3392
_cell_measurement_temperature    298
_cell_measurement_theta_max      24.24
_cell_measurement_theta_min      2.27
_cell_volume                     4021(3)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_diffrn_ambient_temperature      298
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.710
_diffrn_reflns_av_R_equivalents  0.0714
_diffrn_reflns_av_unetI/netI     0.0871
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_number            26931
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.214
_diffrn_reflns_theta_max         27.221
_diffrn_reflns_theta_min         1.551
_exptl_absorpt_coefficient_mu    2.442
_exptl_absorpt_correction_T_max  0.732
_exptl_absorpt_correction_T_min  0.707
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            'clear dark green'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   dark
_exptl_crystal_colour_primary    green
_exptl_crystal_density_diffrn    2.390
_exptl_crystal_description       block
_exptl_crystal_F_000             2786
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.1
_refine_diff_density_max         2.766
_refine_diff_density_min         -1.937
_refine_diff_density_rms         0.185
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.032
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     589
_refine_ls_number_reflns         8948
_refine_ls_number_restraints     23
_refine_ls_restrained_S_all      1.041
_refine_ls_R_factor_all          0.1111
_refine_ls_R_factor_gt           0.0608
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0644P)²+12.4015P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1333
_refine_ls_wR_factor_ref         0.1535
_reflns_Friedel_coverage         0.000
_reflns_number_gt                5628
_reflns_number_total             8948
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c9dt02420d2.cif
_cod_data_source_block           pmo2
_cod_depositor_comments
'Adding full bibliography for 7700697--7700698.cif.'
_cod_database_code               7700698
_shelxl_version_number           2014-1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups
2. Restrained distances
 C1-C2
 2.1 with sigma of 0.02
 C1-C2
 2.1 with sigma of 0.02
 C1-C2
 2.2 with sigma of 0.02
 C1-C2
 2.1 with sigma of 0.02
 C5-C4
 2.1 with sigma of 0.02
3. Uiso/Uaniso restraints and constraints
Uanis(O5) \\sim Ueq, Uanis(O11) \\sim Ueq, Uanis(Mo5) \\sim Ueq: with sigma of
0.01 and sigma for terminal atoms of 0.02
4. Others
 Fixed Sof: O1A(0.5) O1B(0.5) O2A(0.5) O2B(0.5)
5.a Secondary CH2 refined with riding coordinates:
 C3(H3A,H3B), C6(H6A,H6B), C15(H15A,H15B), C21(H21A,H21B)
5.b Aromatic/amide H refined with riding coordinates:
 C1(H1), C2(H2), C4(H4), C5(H5), C8(H8), C9(H9), C11(H11), C12(H12), C13(H13),
 C14(H14), C17(H17), C18(H18), C19(H19), C20(H20), C23(H23), C24(H24)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
P P 0.5000 0.5000 0.0000 0.0234(6) Uani 1 2 d S T P
Mo1 Mo 0.41081(8) 0.42088(5) 0.11832(3) 0.0359(2) Uani 1 1 d . . .
Mo2 Mo 0.30933(8) 0.31550(5) -0.01785(3) 0.0361(2) Uani 1 1 d . . .
Mo3 Mo 0.18202(10) 0.51217(8) 0.00192(4) 0.0629(3) Uani 1 1 d . . .
Mo4 Mo 0.26585(9) 0.60749(5) -0.11175(4) 0.0461(2) Uani 1 1 d . . .
Mo5 Mo 0.36954(9) 0.69275(5) 0.02924(3) 0.0404(2) Uani 1 1 d . U .
Mo6 Mo 0.62044(7) 0.59320(4) 0.13898(3) 0.02933(19) Uani 1 1 d . . .
Cu Cu 0.36629(10) 0.25588(6) 0.23183(4) 0.0281(2) Uani 1 1 d . . .
O1 O 0.3746(8) 0.3729(4) 0.1730(2) 0.0539(19) Uani 1 1 d . . .
O1A O 0.4005(11) 0.4499(7) 0.0175(4) 0.027(2) Uani 0.5 1 d . . .
O1B O 0.4641(9) 0.4220(6) -0.0319(4) 0.018(2) Uani 0.5 1 d . . .
O2 O 0.5826(7) 0.3720(4) 0.1295(4) 0.078(3) Uani 1 1 d . . .
O2A O 0.3787(10) 0.5612(6) -0.0142(4) 0.022(2) Uani 0.5 1 d . . .
O2B O 0.5410(9) 0.4871(6) 0.0655(4) 0.019(2) Uani 0.5 1 d . . .
O3 O 0.3577(7) 0.3293(5) 0.0613(3) 0.066(2) Uani 1 1 d . . .
O4 O 0.2619(8) 0.4724(5) 0.0809(3) 0.068(2) Uani 1 1 d . . .
O5 O 0.4926(7) 0.5168(5) 0.1512(4) 0.076(2) Uani 1 1 d . U .
O6 O 0.2201(8) 0.2301(5) -0.0275(3) 0.075(3) Uani 1 1 d . . .
O7 O 0.1826(7) 0.4009(5) -0.0257(3) 0.066(2) Uani 1 1 d . . .
O8 O 0.0000 0.5000 0.0000 0.096(5) Uani 1 2 d S T P
O9 O 0.1612(10) 0.5547(6) -0.0733(3) 0.094(3) Uani 1 1 d . . .
O10 O 0.2367(10) 0.6236(6) 0.0326(3) 0.094(4) Uani 1 1 d . . .
O11 O 0.3078(10) 0.6900(6) -0.0550(3) 0.088(3) Uani 1 1 d . U .
O12 O 0.1596(6) 0.6541(4) -0.1659(3) 0.0476(17) Uani 1 1 d . . .
O13 O 0.3182(7) 0.7860(4) 0.0425(3) 0.060(2) Uani 1 1 d . . .
O14 O 0.5287(7) 0.7277(5) 0.0159(3) 0.057(2) Uani 1 1 d . . .
O15 O 0.4699(7) 0.6597(5) 0.1025(3) 0.056(2) Uani 1 1 d . . .
O16 O 0.7069(7) 0.6534(5) 0.0991(3) 0.054(2) Uani 1 1 d . . .
O17 O 0.6658(6) 0.6387(5) 0.2045(2) 0.0503(18) Uani 1 1 d . . .
O18 O 0.7265(7) 0.5033(4) 0.1470(4) 0.075(3) Uani 1 1 d . . .
C1 C 0.1777(10) 0.3874(7) 0.2383(4) 0.057(3) Uani 1 1 d D . .
H1 H 0.1603 0.3987 0.1987 0.069 Uiso 1 1 calc R . .
C2 C 0.2555(15) 0.3383(8) 0.3222(4) 0.092(5) Uani 1 1 d D . .
H2 H 0.3047 0.3070 0.3535 0.111 Uiso 1 1 calc R . .
C3 C 0.0245(10) 0.4903(6) 0.2599(4) 0.048(3) Uani 1 1 d . . .
H3A H 0.0126 0.5103 0.2959 0.058 Uiso 1 1 calc R . .
H3B H -0.0560 0.4666 0.2364 0.058 Uiso 1 1 calc R . .
C4 C 0.6306(9) 0.2508(5) 0.3116(4) 0.038(2) Uani 1 1 d D . .
H4 H 0.6347 0.1927 0.3107 0.046 Uiso 1 1 calc R . .
C5 C 0.5668(12) 0.3725(6) 0.3015(6) 0.090(5) Uani 1 1 d D . .
H5 H 0.5129 0.4186 0.2911 0.108 Uiso 1 1 calc R . .
C6 C 0.8626(10) 0.2764(7) 0.3645(4) 0.058(3) Uani 1 1 d . . .
H6A H 0.8758 0.2626 0.4051 0.070 Uiso 1 1 calc R . .
H6B H 0.9186 0.3226 0.3627 0.070 Uiso 1 1 calc R . .
C7 C 0.8926(8) 0.2019(6) 0.3327(4) 0.038(2) Uani 1 1 d . . .
C8 C 0.9342(11) 0.1270(7) 0.3611(4) 0.057(3) Uani 1 1 d . . .
H8 H 0.9433 0.1223 0.4006 0.069 Uiso 1 1 calc R . .
C9 C 0.9614(11) 0.0612(7) 0.3323(4) 0.054(3) Uani 1 1 d . . .
H9 H 0.9950 0.0130 0.3529 0.065 Uiso 1 1 calc R . .
C10 C 0.9407(9) 0.0633(6) 0.2724(4) 0.042(2) Uani 1 1 d . . .
C11 C 0.8926(9) 0.1364(6) 0.2439(4) 0.042(2) Uani 1 1 d . . .
H11 H 0.8749 0.1392 0.2037 0.050 Uiso 1 1 calc R . .
C12 C 0.8706(10) 0.2042(6) 0.2729(4) 0.050(3) Uani 1 1 d . . .
H12 H 0.8403 0.2532 0.2525 0.060 Uiso 1 1 calc R . .
C13 C 0.4834(14) 0.0935(6) 0.2058(5) 0.072(4) Uani 1 1 d . . .
H13 H 0.4567 0.0662 0.2342 0.087 Uiso 1 1 calc R . .
C14 C 0.5208(9) 0.1875(5) 0.1541(4) 0.037(2) Uani 1 1 d . . .
H14 H 0.5258 0.2389 0.1368 0.045 Uiso 1 1 calc R . .
C15 C 0.6369(10) 0.1006(6) 0.0988(4) 0.047(3) Uani 1 1 d . . .
H15A H 0.7168 0.0726 0.1184 0.056 Uiso 1 1 calc R . .
H15B H 0.6578 0.1536 0.0843 0.056 Uiso 1 1 calc R . .
C16 C 0.5646(10) 0.0483(5) 0.0482(4) 0.035(2) Uani 1 1 d . . .
C17 C 0.4476(12) 0.0694(7) 0.0133(4) 0.059(3) Uani 1 1 d . . .
H17 H 0.4087 0.1170 0.0225 0.070 Uiso 1 1 calc R . .
C18 C 0.6170(11) -0.0244(6) 0.0350(4) 0.053(3) Uani 1 1 d . . .
H18 H 0.6959 -0.0429 0.0587 0.064 Uiso 1 1 calc R . .
C19 C 0.1121(11) 0.1766(8) 0.1839(4) 0.062(3) Uani 1 1 d . . .
H19 H 0.1120 0.1632 0.2215 0.075 Uiso 1 1 calc R . .
C20 C 0.1696(9) 0.2239(6) 0.1160(4) 0.040(2) Uani 1 1 d . . .
H20 H 0.2154 0.2503 0.0942 0.047 Uiso 1 1 calc R . .
C21 C -0.0145(10) 0.1728(6) 0.0337(4) 0.043(2) Uani 1 1 d . . .
H21A H 0.0178 0.2088 0.0089 0.052 Uiso 1 1 calc R . .
H21B H -0.1036 0.1870 0.0279 0.052 Uiso 1 1 calc R . .
C22 C -0.0052(10) 0.0822(6) 0.0166(4) 0.042(2) Uani 1 1 d . . .
C23 C -0.1123(10) 0.0421(7) -0.0161(5) 0.064(3) Uani 1 1 d . . .
H23 H -0.1900 0.0703 -0.0278 0.077 Uiso 1 1 calc R . .
C24 C 0.1062(11) 0.0392(8) 0.0320(6) 0.073(4) Uani 1 1 d . . .
H24 H 0.1805 0.0659 0.0539 0.087 Uiso 1 1 calc R . .
N1 N 0.2623(7) 0.3305(4) 0.2679(3) 0.0350(17) Uani 1 1 d . . .
N2 N 0.1722(13) 0.3946(7) 0.3264(4) 0.098(5) Uani 1 1 d . . .
N3 N 0.1230(8) 0.4249(5) 0.2731(3) 0.0406(19) Uani 1 1 d . . .
N4 N 0.5278(7) 0.2948(4) 0.2881(3) 0.0318(16) Uani 1 1 d . . .
N5 N 0.6890(11) 0.3786(5) 0.3310(5) 0.091(4) Uani 1 1 d . . .
N6 N 0.7281(8) 0.3004(5) 0.3368(3) 0.044(2) Uani 1 1 d . . .
N7 N 0.4642(7) 0.1747(4) 0.1952(3) 0.0332(17) Uani 1 1 d . . .
N8 N 0.5682(8) 0.1172(4) 0.1415(3) 0.0394(19) Uani 1 1 d . . .
N9 N 0.5426(12) 0.0544(6) 0.1735(4) 0.084(4) Uani 1 1 d . . .
N10 N 0.2067(7) 0.2181(4) 0.1731(3) 0.0314(16) Uani 1 1 d . . .
N11 N 0.0183(9) 0.1558(6) 0.1377(3) 0.063(3) Uani 1 1 d . . .
N12 N 0.0585(8) 0.1870(5) 0.0943(3) 0.0381(18) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0030 0.0020 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0060 0.0030 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0110 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1020 0.0940 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1A P O1A 180.0(6) 3_665 .
O1A P O2A 103.8(5) . 3_665
O1A P O2A 76.2(5) . .
O1A P O2A 76.2(5) 3_665 3_665
O1A P O2A 103.8(5) 3_665 .
O1A P O2B 110.4(5) . 3_665
O1A P O2B 69.6(5) . .
O1A P O2B 110.4(5) 3_665 .
O1A P O2B 69.6(5) 3_665 3_665
O1B P O1A 114.2(5) . 3_665
O1B P O1A 114.2(5) 3_665 .
O1B P O1A 65.8(5) 3_665 3_665
O1B P O1A 65.8(5) . .
O1B P O1B 180.0 3_665 .
O1B P O2A 109.6(5) . .
O1B P O2A 70.4(5) 3_665 .
O1B P O2A 109.6(5) 3_665 3_665
O1B P O2A 70.4(5) . 3_665
O1B P O2B 112.4(5) . .
O1B P O2B 112.4(5) 3_665 3_665
O1B P O2B 67.6(5) 3_665 .
O1B P O2B 67.6(5) . 3_665
O2A P O2A 180.0 3_665 .
O2B P O2A 74.2(5) . 3_665
O2B P O2A 74.2(5) 3_665 .
O2B P O2A 105.8(5) . .
O2B P O2A 105.8(5) 3_665 3_665
O2B P O2B 180.0 3_665 .
O1 Mo1 O1A 156.9(3) . .
O1 Mo1 O2 98.8(4) . .
O1 Mo1 O2B 158.6(4) . .
O1 Mo1 O3 96.8(3) . .
O1 Mo1 O4 102.1(4) . .
O1 Mo1 O5 104.2(4) . .
O2 Mo1 O1A 88.2(4) . .
O2 Mo1 O2B 63.8(3) . .
O2B Mo1 O1A 41.7(3) . .
O3 Mo1 O1A 62.1(3) . .
O3 Mo1 O2 82.6(3) . .
O3 Mo1 O2B 93.2(3) . .
O4 Mo1 O1A 69.6(3) . .
O4 Mo1 O2 157.8(4) . .
O4 Mo1 O2B 97.2(4) . .
O4 Mo1 O3 87.5(3) . .
O4 Mo1 O5 94.9(4) . .
O5 Mo1 O1A 98.1(4) . .
O5 Mo1 O2 87.1(3) . .
O5 Mo1 O2B 64.6(4) . .
O5 Mo1 O3 157.8(4) . .
O1A Mo2 O1B 38.2(3) . .
O3 Mo2 O1A 64.3(3) . .
O3 Mo2 O1B 93.6(3) . .
O3 Mo2 O7 89.5(3) . .
O3 Mo2 O14 92.4(3) . 3_665
O3 Mo2 O16 155.9(4) . 3_665
O6 Mo2 O1A 161.5(4) . .
O6 Mo2 O1B 160.1(4) . .
O6 Mo2 O3 102.7(4) . .
O6 Mo2 O7 101.2(4) . .
O6 Mo2 O14 102.3(4) . 3_665
O6 Mo2 O16 101.2(4) . 3_665
O7 Mo2 O1A 67.2(4) . .
O7 Mo2 O1B 90.1(3) . .
O7 Mo2 O16 82.9(3) . 3_665
O14 Mo2 O1A 91.7(4) 3_665 .
O14 Mo2 O1B 65.3(3) 3_665 .
O14 Mo2 O7 155.4(4) 3_665 .
O14 Mo2 O16 85.5(3) 3_665 3_665
O16 Mo2 O1A 91.7(3) 3_665 .
O16 Mo2 O1B 63.7(3) 3_665 .
O2A Mo3 O1A 45.7(3) . .
O4 Mo3 O1A 66.2(3) . .
O4 Mo3 O2A 95.8(3) . .
O4 Mo3 O8 98.3(3) . .
O4 Mo3 O10 86.0(3) . .
O7 Mo3 O1A 65.1(3) . .
O7 Mo3 O2A 98.6(3) . .
O7 Mo3 O4 89.4(3) . .
O7 Mo3 O8 90.5(3) . .
O7 Mo3 O10 162.5(4) . .
O8 Mo3 O1A 150.1(2) . .
O8 Mo3 O2A 163.3(2) . .
O9 Mo3 O1A 97.0(4) . .
O9 Mo3 O2A 65.7(4) . .
O9 Mo3 O4 161.2(4) . .
O9 Mo3 O7 90.7(3) . .
O9 Mo3 O8 100.5(3) . .
O9 Mo3 O10 88.3(3) . .
O10 Mo3 O1A 97.7(4) . .
O10 Mo3 O2A 65.2(4) . .
O10 Mo3 O8 106.8(3) . .
O2 Mo4 O2A 92.6(4) 3_665 .
O2 Mo4 O9 155.6(4) 3_665 .
O2 Mo4 O18 84.5(3) 3_665 3_665
O9 Mo4 O2A 66.0(4) . .
O9 Mo4 O18 85.4(4) . 3_665
O11 Mo4 O2 90.2(4) . 3_665
O11 Mo4 O2A 64.0(4) . .
O11 Mo4 O9 90.5(3) . .
O11 Mo4 O18 157.0(4) . 3_665
O12 Mo4 O2 101.9(4) . 3_665
O12 Mo4 O2A 160.6(3) . .
O12 Mo4 O9 101.7(4) . .
O12 Mo4 O11 102.8(4) . .
O12 Mo4 O18 100.1(3) . 3_665
O18 Mo4 O2A 93.9(4) 3_665 .
O10 Mo5 O2A 68.1(4) . .
O10 Mo5 O11 90.1(3) . .
O10 Mo5 O14 159.2(4) . .
O10 Mo5 O15 92.2(3) . .
O11 Mo5 O2A 64.2(4) . .
O11 Mo5 O14 83.2(3) . .
O13 Mo5 O2A 161.3(4) . .
O13 Mo5 O10 102.2(4) . .
O13 Mo5 O11 100.9(4) . .
O13 Mo5 O14 98.4(4) . .
O13 Mo5 O15 102.2(3) . .
O14 Mo5 O2A 91.3(3) . .
O15 Mo5 O2A 94.3(3) . .
O15 Mo5 O11 155.7(4) . .
O15 Mo5 O14 86.2(3) . .
O2B Mo6 O1B 39.5(3) . 3_665
O5 Mo6 O1B 92.0(4) . 3_665
O5 Mo6 O2B 63.4(3) . .
O15 Mo6 O1B 65.2(3) . 3_665
O15 Mo6 O2B 89.0(3) . .
O15 Mo6 O5 81.9(3) . .
O16 Mo6 O1B 65.9(3) . 3_665
O16 Mo6 O2B 96.6(3) . .
O16 Mo6 O5 157.9(4) . .
O16 Mo6 O15 88.7(3) . .
O16 Mo6 O18 93.3(3) . .
O17 Mo6 O1B 159.7(3) . 3_665
O17 Mo6 O2B 159.4(3) . .
O17 Mo6 O5 98.9(4) . .
O17 Mo6 O15 99.2(3) . .
O17 Mo6 O16 102.4(3) . .
O17 Mo6 O18 104.1(4) . .
O18 Mo6 O1B 93.5(4) . 3_665
O18 Mo6 O2B 66.6(4) . .
O18 Mo6 O5 87.4(3) . .
O18 Mo6 O15 155.6(4) . .
N1 Cu O1 85.3(3) . .
N1 Cu N7 176.6(3) . .
N4 Cu O1 88.5(3) . .
N4 Cu N1 91.4(3) . .
N4 Cu N7 91.0(3) . .
N4 Cu N10 178.0(3) . .
N7 Cu O1 97.1(3) . .
N10 Cu O1 89.9(3) . .
N10 Cu N1 89.8(3) . .
N10 Cu N7 87.9(3) . .
Mo1 O1 Cu 153.6(4) . .
P O1A Mo1 123.8(6) . .
P O1A Mo2 129.0(5) . .
P O1A Mo3 118.9(6) . .
P O1A O1B 55.5(5) . .
P O1A O2B 55.5(5) . .
Mo1 O1A Mo3 88.9(3) . .
Mo2 O1A Mo1 94.1(4) . .
Mo2 O1A Mo3 91.4(4) . .
O1B O1A Mo1 141.3(7) . .
O1B O1A Mo2 73.6(5) . .
O1B O1A Mo3 127.1(6) . .
O1B O1A O2B 95.4(7) . .
O2B O1A Mo1 68.5(4) . .
O2B O1A Mo2 137.1(6) . .
O2B O1A Mo3 125.4(6) . .
P O1B Mo2 126.9(5) . .
P O1B Mo6 126.2(5) . 3_665
P O1B O1A 58.8(5) . .
P O1B O2A 58.7(5) . 3_665
P O1B O2B 58.1(5) . 3_665
Mo6 O1B Mo2 91.0(3) 3_665 .
O1A O1B Mo2 68.1(5) . .
O1A O1B Mo6 133.4(6) . 3_665
O1A O1B O2A 92.9(7) . 3_665
O1A O1B O2B 99.2(7) . 3_665
O2A O1B Mo2 126.4(5) 3_665 .
O2A O1B Mo6 131.1(6) 3_665 3_665
O2B O1B Mo2 137.7(6) 3_665 .
O2B O1B Mo6 68.2(4) 3_665 3_665
O2B O1B O2A 93.3(7) 3_665 3_665
Mo4 O2 Mo1 140.8(4) 3_665 .
P O2A Mo3 119.2(5) . .
P O2A Mo4 122.9(5) . .
P O2A Mo5 126.3(5) . .
P O2A O1B 50.9(4) . 3_665
Mo4 O2A Mo3 92.0(3) . .
Mo5 O2A Mo3 93.4(4) . .
Mo5 O2A Mo4 94.6(3) . .
O1B O2A Mo3 133.9(6) 3_665 .
O1B O2A Mo4 132.9(6) 3_665 .
O1B O2A Mo5 75.5(5) 3_665 .
P O2B Mo1 124.6(5) . .
P O2B Mo6 126.5(5) . .
P O2B O1A 54.9(4) . .
P O2B O1B 54.3(4) . 3_665
Mo6 O2B Mo1 93.6(3) . .
O1A O2B Mo1 69.8(4) . .
O1A O2B Mo6 141.6(6) . .
O1B O2B Mo1 134.6(6) 3_665 .
O1B O2B Mo6 72.2(4) 3_665 .
O1B O2B O1A 94.7(7) 3_665 .
Mo2 O3 Mo1 138.3(5) . .
Mo1 O4 Mo3 135.2(4) . .
Mo1 O5 Mo6 137.8(5) . .
Mo3 O7 Mo2 135.3(4) . .
Mo3 O8 Mo3 180.0 . 3_565
Mo4 O9 Mo3 136.2(5) . .
Mo5 O10 Mo3 133.2(6) . .
Mo4 O11 Mo5 136.0(5) . .
Mo2 O14 Mo5 140.4(4) 3_665 .
Mo5 O15 Mo6 140.3(4) . .
Mo6 O16 Mo2 138.8(4) . 3_665
Mo6 O18 Mo4 140.2(5) . 3_665
N1 C1 H1 124.9 . .
N3 C1 H1 124.9 . .
N3 C1 N1 110.1(7) . .
N1 C2 H2 123.7 . .
N2 C2 H2 123.7 . .
N2 C2 N1 112.6(8) . .
H3A C3 H3B 107.9 . .
C10 C3 H3A 109.2 2_655 .
C10 C3 H3B 109.2 2_655 .
N3 C3 H3A 109.2 . .
N3 C3 H3B 109.2 . .
N3 C3 C10 112.2(8) . 2_655
N4 C4 H4 124.8 . .
N4 C4 N6 110.5(8) . .
N6 C4 H4 124.8 . .
N4 C5 H5 123.1 . .
N5 C5 H5 123.1 . .
N5 C5 N4 113.7(9) . .
H6A C6 H6B 108.4 . .
C7 C6 H6A 110.0 . .
C7 C6 H6B 110.0 . .
N6 C6 H6A 110.0 . .
N6 C6 H6B 110.0 . .
N6 C6 C7 108.4(8) . .
C8 C7 C6 121.6(9) . .
C8 C7 C12 117.6(9) . .
C12 C7 C6 120.6(9) . .
C7 C8 H8 119.5 . .
C9 C8 C7 120.9(9) . .
C9 C8 H8 119.5 . .
C8 C9 H9 119.2 . .
C8 C9 C10 121.6(10) . .
C10 C9 H9 119.2 . .
C9 C10 C3 121.7(9) . 2_645
C11 C10 C3 121.1(8) . 2_645
C11 C10 C9 117.1(10) . .
C10 C11 H11 119.2 . .
C12 C11 C10 121.6(9) . .
C12 C11 H11 119.2 . .
C7 C12 H12 119.6 . .
C11 C12 C7 120.9(9) . .
C11 C12 H12 119.6 . .
N7 C13 H13 122.3 . .
N9 C13 H13 122.3 . .
N9 C13 N7 115.5(9) . .
N7 C14 H14 124.9 . .
N8 C14 H14 124.9 . .
N8 C14 N7 110.3(8) . .
H15A C15 H15B 107.6 . .
C16 C15 H15A 108.6 . .
C16 C15 H15B 108.6 . .
N8 C15 H15A 108.6 . .
N8 C15 H15B 108.6 . .
N8 C15 C16 114.5(8) . .
C17 C16 C15 122.7(8) . .
C17 C16 C18 117.0(9) . .
C18 C16 C15 120.3(9) . .
C16 C17 H17 118.4 . .
C16 C17 C18 123.3(9) . 3_655
C18 C17 H17 118.4 3_655 .
C16 C18 H18 120.2 . .
C17 C18 C16 119.7(10) 3_655 .
C17 C18 H18 120.2 3_655 .
N10 C19 H19 122.5 . .
N11 C19 H19 122.5 . .
N11 C19 N10 114.9(8) . .
N10 C20 H20 125.0 . .
N12 C20 H20 125.0 . .
N12 C20 N10 110.1(8) . .
H21A C21 H21B 108.0 . .
C22 C21 H21A 109.4 . .
C22 C21 H21B 109.4 . .
N12 C21 H21A 109.4 . .
N12 C21 H21B 109.4 . .
N12 C21 C22 111.1(8) . .
C23 C22 C21 119.4(9) . .
C24 C22 C21 122.7(9) . .
C24 C22 C23 117.9(10) . .
C22 C23 H23 119.8 . .
C24 C23 C22 120.4(10) 3 .
C24 C23 H23 119.8 3 .
C22 C24 C23 121.6(10) . 3
C22 C24 H24 119.2 . .
C23 C24 H24 119.2 3 .
C1 N1 Cu 124.1(6) . .
C2 N1 Cu 132.9(7) . .
C2 N1 C1 103.1(7) . .
C2 N2 N3 105.5(8) . .
C1 N3 C3 129.4(8) . .
C1 N3 N2 108.7(8) . .
N2 N3 C3 121.9(8) . .
C4 N4 Cu 127.3(6) . .
C4 N4 C5 103.1(8) . .
C5 N4 Cu 128.3(7) . .
N6 N5 C5 103.5(8) . .
C4 N6 C6 127.8(9) . .
N5 N6 C4 109.1(8) . .
N5 N6 C6 123.0(9) . .
C13 N7 Cu 127.6(6) . .
C13 N7 C14 102.1(8) . .
C14 N7 Cu 130.2(6) . .
C14 N8 C15 129.7(8) . .
C14 N8 N9 109.9(7) . .
N9 N8 C15 120.3(8) . .
C13 N9 N8 102.1(8) . .
C19 N10 Cu 126.1(6) . .
C20 N10 Cu 130.8(6) . .
C20 N10 C19 103.1(7) . .
C19 N11 N12 102.1(8) . .
C20 N12 C21 129.3(8) . .
C20 N12 N11 109.8(7) . .
N11 N12 C21 120.7(8) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
P O1A 1.510(11) 3_665
P O1A 1.510(10) .
P O1B 1.454(10) 3_665
P O1B 1.454(10) .
P O2A 1.601(10) 3_665
P O2A 1.601(10) .
P O2B 1.520(9) .
P O2B 1.520(9) 3_665
Mo1 O1 1.672(6) .
Mo1 O1A 2.441(9) .
Mo1 O2 1.980(7) .
Mo1 O2B 2.420(9) .
Mo1 O3 1.972(7) .
Mo1 O4 1.808(7) .
Mo1 O5 1.831(8) .
Mo2 O1A 2.414(11) .
Mo2 O1B 2.496(10) .
Mo2 O3 1.831(6) .
Mo2 O6 1.654(7) .
Mo2 O7 1.915(7) .
Mo2 O14 1.891(7) 3_665
Mo2 O16 1.974(6) 3_665
Mo3 O1A 2.514(11) .
Mo3 O2A 2.430(10) .
Mo3 O4 1.946(7) .
Mo3 O7 1.899(7) .
Mo3 O8 1.9898(15) .
Mo3 O9 1.883(7) .
Mo3 O10 1.953(8) .
Mo4 O2 1.863(8) 3_665
Mo4 O2A 2.420(9) .
Mo4 O9 1.876(8) .
Mo4 O11 1.855(8) .
Mo4 O12 1.642(6) .
Mo4 O18 1.977(7) 3_665
Mo5 O2A 2.364(10) .
Mo5 O10 1.848(8) .
Mo5 O11 1.937(7) .
Mo5 O13 1.657(6) .
Mo5 O14 1.947(8) .
Mo5 O15 1.853(6) .
Mo6 O1B 2.477(8) 3_665
Mo6 O2B 2.416(9) .
Mo6 O5 1.946(8) .
Mo6 O15 1.937(6) .
Mo6 O16 1.814(6) .
Mo6 O17 1.672(5) .
Mo6 O18 1.821(7) .
Cu O1 2.364(6) .
Cu N1 2.018(7) .
Cu N4 1.978(7) .
Cu N7 2.044(7) .
Cu N10 1.984(7) .
O1A O1B 1.610(13) .
O1A O2B 1.729(14) .
O1B Mo6 2.477(8) 3_665
O1B O2A 1.766(13) 3_665
O1B O2B 1.656(13) 3_665
O2 Mo4 1.863(8) 3_665
O2A O1B 1.766(13) 3_665
O2B O1B 1.656(13) 3_665
O8 Mo3 1.9898(15) 3_565
O14 Mo2 1.891(7) 3_665
O16 Mo2 1.974(6) 3_665
O18 Mo4 1.977(7) 3_665
C1 H1 0.9300 .
C1 N1 1.342(11) .
C1 N3 1.311(12) .
C2 H2 0.9300 .
C2 N1 1.335(11) .
C2 N2 1.308(14) .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
C3 C10 1.513(13) 2_655
C3 N3 1.467(11) .
C4 H4 0.9300 .
C4 N4 1.303(11) .
C4 N6 1.322(12) .
C5 H5 0.9300 .
C5 N4 1.322(12) .
C5 N5 1.317(14) .
C6 H6A 0.9700 .
C6 H6B 0.9700 .
C6 C7 1.504(13) .
C6 N6 1.473(13) .
C7 C8 1.385(14) .
C7 C12 1.388(12) .
C8 H8 0.9300 .
C8 C9 1.342(14) .
C9 H9 0.9300 .
C9 C10 1.393(13) .
C10 C3 1.513(13) 2_645
C10 C11 1.377(13) .
C11 H11 0.9300 .
C11 C12 1.349(13) .
C12 H12 0.9300 .
C13 H13 0.9300 .
C13 N7 1.327(12) .
C13 N9 1.311(12) .
C14 H14 0.9300 .
C14 N7 1.332(10) .
C14 N8 1.311(11) .
C15 H15A 0.9700 .
C15 H15B 0.9700 .
C15 C16 1.494(13) .
C15 N8 1.468(10) .
C16 C17 1.347(14) .
C16 C18 1.374(12) .
C17 H17 0.9300 .
C17 C18 1.371(14) 3_655
C18 C17 1.371(14) 3_655
C18 H18 0.9300 .
C19 H19 0.9300 .
C19 N10 1.319(11) .
C19 N11 1.311(12) .
C20 H20 0.9300 .
C20 N10 1.315(10) .
C20 N12 1.311(11) .
C21 H21A 0.9700 .
C21 H21B 0.9700 .
C21 C22 1.516(13) .
C21 N12 1.457(10) .
C22 C23 1.361(13) .
C22 C24 1.352(15) .
C23 H23 0.9300 .
C23 C24 1.361(15) 3
C24 C23 1.361(15) 3
C24 H24 0.9300 .
N2 N3 1.326(11) .
N5 N6 1.316(11) .
N8 N9 1.346(10) .
N11 N12 1.344(10) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
P O1A O1B Mo2 178.5(5) . .
P O1A O1B Mo6 -112.2(8) . 3_665
P O1A O1B O2A 50.3(5) . 3_665
P O1A O1B O2B -43.5(5) . 3_665
P O1A O2B Mo1 175.6(5) . .
P O1A O2B Mo6 106.5(9) . .
P O1A O2B O1B 39.4(5) . 3_665
Mo1 O1A O1B P -102.8(11) . .
Mo1 O1A O1B Mo2 75.7(10) . .
Mo1 O1A O1B Mo6 145.0(7) . 3_665
Mo1 O1A O1B O2A -52.5(12) . 3_665
Mo1 O1A O1B O2B -146.3(9) . 3_665
Mo1 O1A O2B P -175.6(5) . .
Mo1 O1A O2B Mo6 -69.1(8) . .
Mo1 O1A O2B O1B -136.1(6) . 3_665
Mo2 O1A O1B P -178.5(5) . .
Mo2 O1A O1B Mo6 69.3(7) . 3_665
Mo2 O1A O1B O2A -128.3(5) . 3_665
Mo2 O1A O1B O2B 138.0(6) . 3_665
Mo2 O1A O2B P 112.5(9) . .
Mo2 O1A O2B Mo1 -71.9(7) . .
Mo2 O1A O2B Mo6 -141.0(7) . .
Mo2 O1A O2B O1B 151.9(8) . 3_665
Mo3 O1A O1B P 102.4(7) . .
Mo3 O1A O1B Mo2 -79.1(7) . .
Mo3 O1A O1B Mo6 -9.8(13) . 3_665
Mo3 O1A O1B O2A 152.7(7) . 3_665
Mo3 O1A O1B O2B 58.9(9) . 3_665
Mo3 O1A O2B P -103.3(7) . .
Mo3 O1A O2B Mo1 72.3(5) . .
Mo3 O1A O2B Mo6 3.2(13) . .
Mo3 O1A O2B O1B -63.9(8) . 3_665
O1 Mo1 O4 Mo3 -155.7(6) . .
O1 Mo1 O5 Mo6 152.5(7) . .
O1A P O1B Mo2 178.3(6) 3_665 .
O1A P O1B Mo2 -1.7(6) . .
O1A P O1B Mo6 -56.6(8) 3_665 3_665
O1A P O1B Mo6 123.4(8) . 3_665
O1A P O1B O1A 179.998(1) 3_665 .
O1A P O1B O2A -116.0(6) . 3_665
O1A P O1B O2A 64.0(6) 3_665 3_665
O1A P O1B O2B 126.8(6) . 3_665
O1A P O1B O2B -53.2(6) 3_665 3_665
O1A P O2A Mo3 177.7(5) 3_665 .
O1A P O2A Mo3 -2.3(5) . .
O1A P O2A Mo4 -116.3(7) . .
O1A P O2A Mo4 63.7(7) 3_665 .
O1A P O2A Mo5 117.3(7) . .
O1A P O2A Mo5 -62.7(7) 3_665 .
O1A P O2A O1B 122.4(5) . 3_665
O1A P O2A O1B -57.6(5) 3_665 3_665
O1A P O2B Mo1 174.9(6) 3_665 .
O1A P O2B Mo1 -5.1(6) . .
O1A P O2B Mo6 47.8(8) 3_665 .
O1A P O2B Mo6 -132.2(8) . .
O1A P O2B O1A 180.002(1) 3_665 .
O1A P O2B O1B 51.2(6) 3_665 3_665
O1A P O2B O1B -128.8(6) . 3_665
O1A Mo1 O1 Cu 63.9(15) . .
O1A Mo1 O4 Mo3 1.9(6) . .
O1A Mo1 O5 Mo6 -33.6(7) . .
O1A Mo2 O3 Mo1 11.7(6) . .
O1A Mo3 O7 Mo2 10.7(5) . .
O1A Mo3 O9 Mo4 -39.4(8) . .
O1B P O1A Mo1 -47.2(8) 3_665 .
O1B P O1A Mo1 132.8(8) . .
O1B P O1A Mo2 -178.2(6) 3_665 .
O1B P O1A Mo2 1.8(6) . .
O1B P O1A Mo3 -117.1(7) . .
O1B P O1A Mo3 62.9(7) 3_665 .
O1B P O1A O1B 180.003(1) 3_665 .
O1B P O1A O2B -52.2(6) 3_665 .
O1B P O1A O2B 127.8(6) . .
O1B P O2A Mo3 55.3(6) . .
O1B P O2A Mo3 -124.7(6) 3_665 .
O1B P O2A Mo4 -58.7(7) . .
O1B P O2A Mo4 121.3(7) 3_665 .
O1B P O2A Mo5 174.9(6) . .
O1B P O2A Mo5 -5.1(6) 3_665 .
O1B P O2A O1B 179.997(1) . 3_665
O1B P O2B Mo1 -56.3(7) . .
O1B P O2B Mo1 123.7(7) 3_665 .
O1B P O2B Mo6 -3.4(6) 3_665 .
O1B P O2B Mo6 176.6(6) . .
O1B P O2B O1A 128.8(6) 3_665 .
O1B P O2B O1A -51.2(6) . .
O1B P O2B O1B 180.000(2) . 3_665
O1B Mo2 O3 Mo1 37.1(7) . .
O1B Mo6 O16 Mo2 8.7(5) 3_665 3_665
O1B Mo6 O18 Mo4 -33.6(7) 3_665 3_665
O1B O1A O2B P 40.8(5) . .
O1B O1A O2B Mo1 -143.6(6) . .
O1B O1A O2B Mo6 147.3(8) . .
O1B O1A O2B O1B 80.3(7) . 3_665
O2 Mo1 O1 Cu -42.4(10) . .
O2 Mo1 O4 Mo3 4.3(14) . .
O2 Mo1 O5 Mo6 54.2(7) . .
O2 Mo4 O9 Mo3 35.9(13) 3_665 .
O2 Mo4 O11 Mo5 -104.9(8) 3_665 .
O2A P O1A Mo1 -108.0(7) . .
O2A P O1A Mo1 72.0(7) 3_665 .
O2A P O1A Mo2 -58.9(8) 3_665 .
O2A P O1A Mo2 121.1(8) . .
O2A P O1A Mo3 2.2(5) . .
O2A P O1A Mo3 -177.8(5) 3_665 .
O2A P O1A O1B -60.7(6) 3_665 .
O2A P O1A O1B 119.3(6) . .
O2A P O1A O2B 67.1(5) 3_665 .
O2A P O1A O2B -112.9(5) . .
O2A P O1B Mo2 -65.7(7) . .
O2A P O1B Mo2 114.3(7) 3_665 .
O2A P O1B Mo6 59.4(7) . 3_665
O2A P O1B Mo6 -120.6(7) 3_665 3_665
O2A P O1B O1A 116.0(6) 3_665 .
O2A P O1B O1A -64.0(6) . .
O2A P O1B O2A 180.000(1) . 3_665
O2A P O1B O2B -117.2(6) 3_665 3_665
O2A P O1B O2B 62.8(6) . 3_665
O2A P O2B Mo1 -116.8(7) 3_665 .
O2A P O2B Mo1 63.2(7) . .
O2A P O2B Mo6 -63.9(7) . .
O2A P O2B Mo6 116.1(7) 3_665 .
O2A P O2B O1A 68.3(6) . .
O2A P O2B O1A -111.7(6) 3_665 .
O2A P O2B O1B -60.5(6) . 3_665
O2A P O2B O1B 119.5(6) 3_665 3_665
O2A Mo3 O7 Mo2 42.6(6) . .
O2A Mo3 O9 Mo4 -5.3(7) . .
O2A Mo4 O9 Mo3 5.3(7) . .
O2A Mo4 O11 Mo5 -12.1(7) . .
O2A Mo5 O10 Mo3 -4.2(6) . .
O2A Mo5 O15 Mo6 39.8(7) . .
O2B P O1A Mo1 5.0(6) . .
O2B P O1A Mo1 -175.0(6) 3_665 .
O2B P O1A Mo2 -126.0(8) . .
O2B P O1A Mo2 54.0(8) 3_665 .
O2B P O1A Mo3 -64.9(7) 3_665 .
O2B P O1A Mo3 115.1(7) . .
O2B P O1A O1B 52.2(6) 3_665 .
O2B P O1A O1B -127.8(6) . .
O2B P O1A O2B 180.001(1) 3_665 .
O2B P O1B Mo2 -128.5(7) 3_665 .
O2B P O1B Mo2 51.5(7) . .
O2B P O1B Mo6 -3.3(6) 3_665 3_665
O2B P O1B Mo6 176.7(6) . 3_665
O2B P O1B O1A 53.2(6) . .
O2B P O1B O1A -126.8(6) 3_665 .
O2B P O1B O2A 117.2(6) 3_665 3_665
O2B P O1B O2A -62.8(6) . 3_665
O2B P O1B O2B 179.998(2) . 3_665
O2B P O2A Mo3 -66.0(6) . .
O2B P O2A Mo3 114.0(6) 3_665 .
O2B P O2A Mo4 179.9(5) . .
O2B P O2A Mo4 -0.1(5) 3_665 .
O2B P O2A Mo5 53.6(7) . .
O2B P O2A Mo5 -126.4(7) 3_665 .
O2B P O2A O1B 58.7(5) . 3_665
O2B P O2A O1B -121.3(5) 3_665 3_665
O2B Mo1 O1 Cu -76.2(13) . .
O2B Mo1 O4 Mo3 33.7(7) . .
O2B Mo1 O5 Mo6 -8.1(6) . .
O2B Mo6 O16 Mo2 34.2(6) . 3_665
O2B Mo6 O18 Mo4 -3.9(6) . 3_665
O2B O1A O1B P -40.8(5) . .
O2B O1A O1B Mo2 137.7(6) . .
O2B O1A O1B Mo6 -153.0(7) . 3_665
O2B O1A O1B O2A 9.4(7) . 3_665
O2B O1A O1B O2B -84.4(7) . 3_665
O3 Mo1 O1 Cu 41.1(10) . .
O3 Mo1 O4 Mo3 -59.2(7) . .
O3 Mo1 O5 Mo6 -8.2(13) . .
O4 Mo1 O1 Cu 130.1(9) . .
O4 Mo1 O5 Mo6 -103.7(7) . .
O4 Mo3 O7 Mo2 -53.2(6) . .
O4 Mo3 O9 Mo4 -14.2(17) . .
O5 Mo1 O1 Cu -131.6(9) . .
O5 Mo1 O4 Mo3 98.7(7) . .
O5 Mo6 O16 Mo2 9.9(12) . 3_665
O5 Mo6 O18 Mo4 58.2(7) . 3_665
O6 Mo2 O3 Mo1 -154.3(7) . .
O7 Mo2 O3 Mo1 -53.0(7) . .
O7 Mo3 O9 Mo4 -104.4(8) . .
O8 Mo3 O7 Mo2 -151.5(5) . .
O8 Mo3 O9 Mo4 164.9(7) . .
O9 Mo3 O7 Mo2 108.1(6) . .
O9 Mo4 O11 Mo5 50.7(8) . .
O10 Mo3 O7 Mo2 21.4(13) . .
O10 Mo3 O9 Mo4 58.1(8) . .
O10 Mo5 O15 Mo6 108.0(7) . .
O11 Mo4 O9 Mo3 -55.7(8) . .
O11 Mo5 O10 Mo3 57.8(7) . .
O11 Mo5 O15 Mo6 13.1(13) . .
O12 Mo4 O9 Mo3 -158.9(7) . .
O12 Mo4 O11 Mo5 152.8(7) . .
O13 Mo5 O10 Mo3 159.0(6) . .
O13 Mo5 O15 Mo6 -149.0(7) . .
O14 Mo2 O3 Mo1 102.5(6) 3_665 .
O14 Mo5 O10 Mo3 -13.0(13) . .
O14 Mo5 O15 Mo6 -51.2(7) . .
O15 Mo5 O10 Mo3 -98.1(6) . .
O15 Mo6 O16 Mo2 -54.6(6) . 3_665
O15 Mo6 O18 Mo4 -5.6(13) . 3_665
O16 Mo2 O3 Mo1 18.2(12) 3_665 .
O16 Mo6 O18 Mo4 -99.7(7) . 3_665
O17 Mo6 O16 Mo2 -153.8(6) . 3_665
O17 Mo6 O18 Mo4 156.6(7) . 3_665
O18 Mo4 O9 Mo3 101.7(8) 3_665 .
O18 Mo4 O11 Mo5 -28.8(14) 3_665 .
O18 Mo6 O16 Mo2 101.0(6) . 3_665
C2 N2 N3 C1 -0.6(16) . .
C2 N2 N3 C3 179.8(11) . .
C3 C10 C11 C12 -174.8(9) 2_645 .
C5 N5 N6 C4 -0.4(15) . .
C5 N5 N6 C6 176.4(11) . .
C6 C7 C8 C9 -179.5(10) . .
C6 C7 C12 C11 -177.4(9) . .
C7 C6 N6 C4 32.6(14) . .
C7 C6 N6 N5 -143.6(11) . .
C7 C8 C9 C10 -4.5(17) . .
C8 C7 C12 C11 -1.8(15) . .
C8 C9 C10 C3 177.9(10) . 2_645
C8 C9 C10 C11 0.9(16) . .
C9 C10 C11 C12 2.3(15) . .
C10 C3 N3 C1 -51.1(14) 2_655 .
C10 C3 N3 N2 128.3(11) 2_655 .
C10 C11 C12 C7 -1.8(16) . .
C12 C7 C8 C9 4.9(16) . .
C14 N8 N9 C13 -2.3(13) . .
C15 C16 C17 C18 176.5(10) . 3_655
C15 C16 C18 C17 -176.6(9) . 3_655
C15 N8 N9 C13 179.4(10) . .
C16 C15 N8 C14 -111.2(11) . .
C16 C15 N8 N9 66.8(13) . .
C17 C16 C18 C17 2.8(17) . 3_655
C18 C16 C17 C18 -2.9(18) . 3_655
C19 N11 N12 C20 -0.4(12) . .
C19 N11 N12 C21 175.7(10) . .
C21 C22 C23 C24 -179.9(11) . 3
C21 C22 C24 C23 180.0(11) . 3
C22 C21 N12 C20 104.4(11) . .
C22 C21 N12 N11 -70.9(12) . .
C23 C22 C24 C23 -1(2) . 3
C24 C22 C23 C24 1(2) . 3
N1 C1 N3 C3 -179.3(9) . .
N1 C1 N3 N2 1.2(14) . .
N1 C2 N2 N3 -0.1(18) . .
N2 C2 N1 Cu -179.0(10) . .
N2 C2 N1 C1 0.8(17) . .
N3 C1 N1 Cu 178.6(6) . .
N3 C1 N1 C2 -1.2(14) . .
N4 C4 N6 C6 -175.3(9) . .
N4 C4 N6 N5 1.3(12) . .
N4 C5 N5 N6 -0.6(18) . .
N5 C5 N4 Cu -166.4(10) . .
N5 C5 N4 C4 1.4(16) . .
N6 C4 N4 Cu 166.3(6) . .
N6 C4 N4 C5 -1.6(12) . .
N6 C6 C7 C8 -121.2(10) . .
N6 C6 C7 C12 54.2(13) . .
N7 C13 N9 N8 3.0(16) . .
N7 C14 N8 C15 179.1(9) . .
N7 C14 N8 N9 1.0(12) . .
N8 C14 N7 Cu -177.3(6) . .
N8 C14 N7 C13 0.7(11) . .
N8 C15 C16 C17 56.3(13) . .
N8 C15 C16 C18 -124.3(10) . .
N9 C13 N7 Cu 175.7(9) . .
N9 C13 N7 C14 -2.4(15) . .
N10 C19 N11 N12 0.2(14) . .
N10 C20 N12 C21 -175.2(9) . .
N10 C20 N12 N11 0.5(12) . .
N11 C19 N10 Cu -177.7(8) . .
N11 C19 N10 C20 0.1(14) . .
N12 C20 N10 Cu 177.3(6) . .
N12 C20 N10 C19 -0.4(11) . .
N12 C21 C22 C23 137.1(10) . .
N12 C21 C22 C24 -43.7(14) . .
